## Abstract

The Dirac equation for relativistic electron waves is the parent model for Weyl and Majorana fermions as well as topological insulators. Simulation of Dirac physics in three-dimensional photonic crystals, though fundamentally important for topological phenomena at optical frequencies, encounters the challenge of synthesis of both Kramers double degeneracy and parity inversion. Here we show how type-II Dirac points—exotic Dirac relativistic waves yet to be discovered—are robustly realized through the nonsymmorphic screw symmetry. The emergent type-II Dirac points carry nontrivial topology and are the mother states of type-II Weyl points. The proposed all-dielectric architecture enables robust cavity states at photonic-crystal—air interfaces and anomalous refraction, with very low energy dissipation.

## Introduction

Dirac’s famous equation for relativistic electron waves^{1} is the foundation for both the quantum field theory and the later topological insulators and semimetals.^{2,3,4} There has been a trend in the simulation of relativistic waves and topological states in classical dynamics such as electromagnetic,^{5, 6} acoustic^{7,8,9} and mechanical waves,^{10, 11} mostly in 2D systems. Many novel phenomena in electromagnetism are discovered along this paradigm, such as photonic *Zitterbewugung*,^{12} zero-index dielectric metamaterials,^{13} deformation induced pseudomagnetic field for photons,^{14} as well as photonic topological insulators with^{15,16,17,18,19} and without^{5, 20,21,22,23,24} time-reversal \(\left( {\cal T} \right)\) symmetry. Recently, such simulation develops from 2D to 3D,^{25,26,27,28,29,30,31,32} exposing to larger wavevector and configuration space that may lead to richer physical phenomena, particularly using \({\cal T}\)-invariant materials which are more feasible for high-frequency (e.g., infrared or visible) applications.

Due to its bosonic nature, i.e., \({{\cal T}^{\rm{2}}}\) = 1, the four-fold degenerate photonic Dirac points (DPs) can be created only when Kramers double degeneracy (“spin”) and parity-inversion (“orbit”) are *synthesized*. These two elements are also at the heart of *Z*
_{2} topology in \({\cal P}{\cal T}\)-symmetric (\({\cal P}\) is inversion) systems, as revealed in the seminal work of Fu and Kane.^{33} Although there have been a few fine designs^{29, 31, 32} showing the connection between type-I DPs and the *Z*
_{2} topology, type-II DPs [in analog of type-II Weyl Points (WPs),^{34, 35} see Fig. 1] have never been explored in photonics or in other classical/bosonic waves. In this work, we demonstrate the creation and destruction of type-II DPs in PhCs. Besides, we unveil screw symmetry, a fundamental type of nonsymmorphic symmetry, as an effective tool for the creation of DPs.

The distinction between symmorphic (e.g., point-group) and nonsymmorphic spatial symmetries in crystals lies in whether the spatial origin can be preserved. Nonsymmorphic symmetries cannot preserve the spatial origin but translate it by a fraction of the crystal period. The screw symmetry, a rotation accompanied with a fraction of lattice translation, is an elementary nonsymmorphic symmetry. So far, the role of screw symmetry on the realization of topological states in classical/bosonic waves has not yet been explored. It is known that screw symmetries lead to double degeneracy for all Bloch states on certain planes in the Brillouin zone (BZ).^{36, 37} Thus the screw symmetries can create a large wavevector space for the simulation of DPs and *Z*
_{2} topology in classical dynamics. The screw symmetries become particularly powerful when there are two orthogonal screw axes, since the product of the two screw rotations is essentially the parity required by the DPs. In this way both the “Kramers” double degeneracy (“spin”) and parity-inversion (“orbit”) can be simultaneously synthesized through screw symmetry.

Based on these symmetry considerations we propose an all-dielectric tetragonal PhC with screw symmetries for the creation of both type-II and type-I DPs. Our symmetry-guided approach is robust: DPs emerge for a variety of geometry and materials. We demonstrate the nontrivial topology of the DPs by studying the edge states. These non-chiral edge states, differing from the chiral edge states of Weyl points (WPs), are below the light-line and form resilient cavity states on PhC-air interfaces. Moreover, we show that both type-II and type-I WPs can be derived from these DPs when symmetry is reduced. Anomalous refraction with one or two pairs of opposite refraction angles is predicted for type-II DPs/WPs. To the best of our knowledge, this is the discovery of type-II DPs in photonics and a proposal of type-II WPs in *all-dielectric* PhCs. Our findings may enable unprecedented control of light at optical frequencies using dissipationless materials.

## Results

### All-dielectric photonic-crystal architecture

We study an all-dielectric PhC with tetragonal symmetry of space group P4_{2}/mcm (see Fig. 2) to illustrate the symmetry-guided approach. In each unit cell, there are two dielectric blocks (painted as yellow and green in Fig. 2) of the same shape and permittivity *ε*
_{
b
}, embedded in a polymer matrix of permittivity *ε*
_{
m
} = 1.9. We shall first set *ε*
_{
b
} = 16 and the geometry parameters *l* = 0.5, *w* = 0.2, and *h* = 0.5 (lattice constant *a* ≡ 1). We show later that DPs emerge for other material/geometric parameters as well. These PhCs can in principle be fabricated using layer-by-layer methods with the current technology^{38, 39} for infrared frequencies. We use the MIT PHOTONIC BANDS (http://ab-initio.mit.edu/wiki/index.php/MITPhotonicBands) to calculate the bulk and surface photonic bands. The tetragonal symmetries crucial to our study are the two-fold screw symmetries \({S_x}: = \left( {x,y,z} \right) \to \left( {\frac{1}{2} + x,\frac{1}{2} - y,\frac{1}{2} - z} \right)\) and \({S_y}: = \left( {x,y,z} \right) \to \left( {\frac{1}{2} - x,\frac{1}{2} + y,\frac{1}{2} - z} \right)\) (illustrated in Fig. 2b), and the 180° rotation around the *z* axis, *C*
_{2}: = (*x*, *y*) → (−*x*, −*y*). The remaining symmetries are listed and analyzed in the Supplementary Materials.

### Photonic Kramers double degeneracy

Anti-unitary operators: \({\Theta _i} \equiv {S_i} * {\cal T}\) (*i* = *x*, *y*) are created to elucidate the power of the screw symmetry. The effect of the time-reversal operation \({\cal T}\) on a photonic Bloch wavefunction \({\Psi _{n\vec k}}\left( {\vec r} \right) = {\left( {{{\vec e}_{n\vec k}},{{\vec h}_{n\vec k}}} \right)^T}\) is mostly complex conjugation, \({\cal T}{\left( {{{\vec e}_{n\vec k}},{{\vec h}_{n\vec k}}} \right)^T} = {\left( {\vec e_{n\vec k}^ * , - \vec h_{n\vec k}^ * } \right)^T}\). Since \(\Theta _x^2 = S_x^2 = {T_{100}}\) where *T*
_{100} is a spatial translation by the vector (1, 0, 0), acting Θ_{
x
} twice on a photonic Bloch state gives \(\Theta _x^2{\Psi _{n\vec k}}\left( {\vec r} \right) = {e^{i{k_x}}}{\Psi _{n\vec k}}\left( {\vec r} \right)\) (see details in Methods). Θ_{
x
} transforms (*k*
_{
x
}, *k*
_{
y
}, *k*
_{
z
}) into (−*k*
_{
x
}, *k*
_{
y
}, *k*
_{
z
}) and is hence invariant on the *k*
_{
x
} = *π* plane, where we find

The above equation, as an analog of the Kramers theorem for fermions, guarantees that *all* photonic states on the *k*
_{
x
} = *π* plane are doubly degenerate (see Fig. 2c). Similarly, all Bloch states are doubly degenerate on the *k*
_{
y
} = *π* plane due to \(\Theta _y^2 = - 1\).

### Dirac points

For the creation of DPs, the next important step is to realize parity-inversion. Here the parity is defined through *C*
_{2}, which is invariant on the MA line, *k*
_{
x
} = *k*
_{
y
} = *π*. The product of the two orthogonal screw rotations yields, *S*
_{
y
}
*S*
_{
x
} = *T*
_{010}
*C*
_{2} and *S*
_{
x
}
*S*
_{
y
} = *T*
_{100}
*C*
_{2}. On the MA line one hence has

Elegantly, the above algebra reveal that the two degenerate states in any doublet have the *same* eigenvalue of the *C*
_{2} rotation. Such eigenvalues *c*
_{2} = ±1 precisely represent the parities of the photonic states in the *x*-*y* plane.

It has been shown in ref. 29 that a DP with synthetic Kramers double degeneracy and parity-inversion has nontrivial topological properties. In fact, such DPs are monopoles of the *SU*(2) Berry-phase gauge fields.^{29} The topological charge of a DP is defined by the integral of the *SU*(2) gauge fields over a tiny sphere containing the DP. It was proved in ref. 40 that in systems with \({\cal P}{\cal T}\) symmetry, the calculation of the topological charge of a DP can be simplified as

where \(c_2^ -\) is the parity of the lower branch of the Dirac cone, and \(k_0^ + = {k_0} + {0^ + }\)
\(\left( {k_0^ - = {k_0} - {0^ + }} \right)\) is the wavevector slightly larger (smaller) than that of the DP on the *z* direction, *k*
_{0}. Since the total topological charge of photonic bands in the BZ is strictly zero, DPs emerge in pairs with opposite *N*
_{
DP
} at opposite wavevectors. Figure 2d shows that there are four DPs in the first six bands, due to the crossing between the *p*- and *d*-doublets.

Our symmetry-guided paradigm provides a robust and effective approach toward topological DPs: Fig. 2e shows that the emergence of DPs is quite robust to the shape and permittivity of the dielectric blocks (more examples are given in the Supplementary Materials), since any crossing between bands of different parities on the MA line leads to DPs.

The spin-orbit physics of the Dirac points can be understood via a symmetry-based \(\vec k\) · \(\vec P\) theory (see Supplementary Materials for details). The Hamiltonian can be constructed using the basis of the two doublets, *p*
_{1}, *p*
_{2}, *d*
_{1} and *d*
_{2} [Fig. 2d]. The combination of these states, \(\left| {{p_ \pm }} \right\rangle = \frac{1}{{\sqrt 2 }}\left( {\left| {{p_1}} \right\rangle \pm i\left| {{p_2}} \right\rangle } \right)\) and \(\left| {{d_ \pm }} \right\rangle = \frac{1}{{\sqrt 2 }}\left( {\left| {{d_1}} \right\rangle \pm i\left| {{d_2}} \right\rangle } \right)\), carry finite total angular momenta (TAM) that are opposite for the + and − states (see Supplementary Materials). Emulating fermionic spin and orbit with the TAM and parity, respectively, we find the following photonic Hamiltonian for a DP,

where *ω*
_{0} is the frequency of the DP, *v* is the characteristic group velocity. \(\hat 1\) is the 2 × 2 identity matrix, \(\widehat {\overrightarrow \sigma }\) is the Pauli matrix vector. The dimensionless \(\vec k\) · \(\vec P\) parameter *η* here plays an role to distinguish the type-I \(\left( {\left| \eta \right| < 1} \right)\) and type-II \(\left( {\left| \eta \right| >1} \right)\) DPs. *g*
_{0} = *iαq*
_{
y
}, *g*
_{
x
} = −*iαq*
_{
x
}, *g*
_{
y
} = *iβq*
_{
x
}, *g*
_{
z
} = −*βq*
_{
y
} with \(\vec q \equiv \vec k - \left( {\pi ,\pi ,{k_0}} \right)\), where *α* and *β* are the (real) \(\vec k\) · \(\vec P\) coefficients, and \({\cal O}\left( {{q^2}} \right)\) denotes the higher-order quadratic warping terms. Here the spin-orbit coupling is emulated by the *k*-linear interaction between the *p* and *d* bands due to quasi-conservation of the TAM.^{29} The 3D Dirac wave can be regarded as a series of *q*
_{
z
}-dependent 2D Dirac waves of which the Dirac mass, *m*
_{
D
} ≡ *vq*
_{
z
}, can be positive, negative, or zero.^{29, 41}

### Derived type-II and type-I Weyl Points

A DP can be regarded as composed of a pair of WPs of opposite Chern numbers. Thus when the space symmetry is reduced WPs can emerge from DPs.^{29} To realize the WPs, we deform the unit-cell structure in such a way (as displayed in Fig. 3a) that the two screw symmetries *S*
_{
x
} and *S*
_{
y
}, the three mirror symmetries *M*
_{1}: = (*x*, *y*) → (*y*, *x*), *M*
_{2}: = (*x*, *y*) → (−*y*, −*x*), and *M*
_{
z
}: = *z* → −*z*, as well as the inversion symmetry \({\cal P}\) are broken. However, the *C*
_{2} symmetry is preserved. The removal of the two screw symmetries lifts the double degeneracy on the MA line. However, accidental degeneracy between bands of opposite parity is protected by the *C*
_{2} symmetry. The chiral structure of the PhC results in *p*
_{±}- and *d*
_{±}-like states in the photonic bands. The crossings between the *p* and *d* bands results in WPs of Chern number ±1 (see Supplementary Materials for a \(\vec k\) · \(\vec P\) analysis). We identify six WPs in Fig. 3b (there are more WPs at higher frequency, explaining the nonzero total Chern number). Figure 3b also shows that there are four type-II WPs and two type-I WPs. The 3D dispersions of both type-I and type-II WPs on the lowest *d*-band are shown in Fig. 3c. Our PhC architecture thus allows realization of type-II WPs using dissipationless all-dielectric materials.

### Robust surface states

According to the bulk-edge correspondence principle,^{2,3,4} the (100) surface states of the tetragonal PhC can reveal the *Z*
_{2} topology of the DPs. We then calculate the surface and projected bulk photonic spectrum using a supercell stacking along the *x* direction [see Methods]. Figure 4a shows a gapless surface band traversing the projected photonic band gap. This surface band is between the upper and lower branches of the type-I DP, but above both branches of the type-II DP. Thus the gapless surface band is induced by the type-I topological DPs. Nonetheless, both type-I and type-II DPs have the same *Z*
_{2} topology (see Fig. 2d). The topological surface states carry finite TAM as indicated in Fig. 4b by the winding profile of the Poynting vectors. The sign of the photonic TAM is changed when the wavevector is reversed (see Fig. 4b). This property is similar to the “spin-wavevector locking” on the edges of topological insulators.^{2, 3} We find that the two symmetries, *S*
_{
y
} and \({\cal T}\), guarantee that the spectrum in the surface BZ is symmetric under the transformation (*k*
_{
y
}, *k*
_{
z
}) → (±*k*
_{
y
}, ±*k*
_{
z
}) (see Methods). It was recently discovered that the surface states of the topological DPs form a double-helicoid surface states with such spectral symmetry. The non-chiral surface bands of our PhC, are distinctive from the chiral surface states due to WPs.^{25, 27, 28} Moreover, the topological surface states here are below the light-line and hence form cavity states on the PhC-air interfaces with no need for additional cladding.

The robustness of the topological surface states can be revealed via their frequency stability against surface modifications. Figure 4c shows that the frequency of the topological surface state is quite robust and insensitive to variations of the thickness of a dielectric slab placed on top of the PhC surface. The change of frequency is within 2.5%, although the field profile has been substantially modified (see Fig. 4d). In contrast, the frequency of a conventional PhC cavity state with woodpile-PhC cladding is much more sensitive to the thickness of the slab^{42} (see inset of Fig. 4c and details in Methods), despite the fact that the woodpile PhC has a large complete photonic band gap of *δω*/*ω* = 21% while our PhC has no complete photonic band gap. The topological surface states thus form resilient, subwavelength quasi-2D photonic systems. The nontrivial topology/Berry-phases and the gapless spectrum distinct them from normal PhC surface states.^{43, 44}

### Spectral and optical properties

Both type-I and type-II DPs appear in Fig. 2. A more careful study is presented in Fig. 5. From Eq. (4), the spectrum of the DPs in the *k*
_{
x
}-*k*
_{
z
} plane (Fig. 5a) is

where *τ* = ± stands for the upper and lower branches of the DP, respectively, the dimensionless parameters \(\gamma = \sqrt {{\alpha ^2} + {\beta ^2}}\) and *η* measure the deformation of the Dirac cone. Particularly, \(\left| \eta \right|\) > 1 for type-II DPs, whereas \(\left| \eta \right|\) < 1 for type-I DPs. The isofrequency contour near a type-II DP is a hyperbolic curve (Fig. 5b). In contrast, the isofrequency contours near a type-I DP is of elliptical shapes. For a type-II DP, when *ω* = *ω*
_{0}, the two branches touch each other and the isofrequency contour becomes a pair of crossing lines (Fig. 5c), between which the angle is \({\theta _{DP}} = 2\,{\rm{arctan}}\left( {\sqrt {\frac{{{\eta ^2} - 1}}{{{\gamma ^2}}}} } \right)\). This quantity sets the bounds on the refraction angles near a type-II DP as \(\pm \frac{1}{2}\left( {\pi - {\theta _{DP}}} \right)\).

The dispersion of the type-II DP in the *k*
_{
x
}-*k*
_{
y
} plane is distinctive from the existing type-I DPs^{29, 31, 32} (see Fig. 5d). This spectrum can be understood via the \(\vec k\) · \(\vec P\) Hamiltonian (4) which yields \({\omega _{\tau ,i}}\left( {\vec q} \right) = {\omega _0} + v\eta {q_z} + v\tau \sqrt {q_z^2 + {\gamma ^2}{{\left| {{q_i}} \right|}^2}} + {\cal O}\left( {{q^2}} \right)\) for *i* = 1, 2, with *τ* = ± and *q*
_{1} = *q*
_{
x
} + *q*
_{
y
} and *q*
_{2} = *q*
_{
y
} − *q*
_{
x
}. This spectrum is nondegenerate for finite *q*
_{
x
} and *q*
_{
y
}. The two-fold degeneracy is restored only when *q*
_{
x
} = 0 or *q*
_{
y
} = 0, in accordance with the screw symmetries. The “V-shaped” dispersion in Fig. 5d gives elliptical-shaped isofrequency contours or non-closing contours in the *k*
_{
x
}-*k*
_{
y
} plane (see Figs. 4f and 5e), depending on the quadratic warping terms.

From the unique spectral properties of the type-II DPs, using frequency and wavevector matching, we derive the anomalous refraction of light: there are two concurrent refraction beams of opposite angles (see schematic in Fig. 5g). An analytic proof is detailed in the Methods section, which is confirmed by the model calculation in Fig. 5h, i for various frequencies, incident angles, and parameters. Interestingly, we find that there is no refraction for *η* > 1, whereas for *η* < −1 there are two refraction beams of opposite refraction angles. Since the two DPs at opposite wavevectors have opposite *η*, the above property can be exploited for *selective excitation* of type-II DPs. Away from the *k*
_{
x
} = *π* and *k*
_{
y
} = *π* planes, the photonic spectrum is nondegenerate, leading to two pairs of beams with opposite refraction angles, as shown in Fig. 5i by varying the angle of incidence *ϕ*
_{
i
} = Arg(*q*
_{
x
} + *iq*
_{
y
}). Zero refraction angle is realized when *ϕ*
_{
i
} is close to \(\frac{\pi }{4},\frac{{3\pi }}{4},\frac{{5\pi }}{4}\), or \(\frac{{7\pi }}{4}\), due to vanishing group velocity in the *k*
_{
x
}-*k*
_{
y
} plane.

The above unconventional optical properties also holds for type-II WPs. Since WPs are two-fold degenerate, there can only be one pair of refraction beams. Concurrent positive and negative refraction was found and confirmed by time-domain simulation in a 2D photonic system before.^{45} Here we find, from frequency-wavevector conservation, that concurrent negative and positive refraction can also be realized in 3D all-dielectric PhCs through type-II DPs/WPs. A time-domain simulation is demanded to further investigate the anomalous refraction, which, however, is beyond the scope of this work.

## Discussion

The band topology induced by crystalline symmetries are in the context of topological crystalline states.^{46, 47} Weak disorders that preserve the crystalline symmetry on average should preserve the DPs and their topological surface states.^{29, 47} The topological surface states here can exist on the PhC-air interface without further cladding, even though such interface does not preserve the screw symmetries. The robustness of the surface photonic bands show superiority over conventional PhC cavity states. This suggests that topology can be a possible tool to suppress inhomogeneous broadening which is a main obstacle for scalable optical and quantum devices. Our all-dielectric topological PhC architecture may inspire future discovery of other 3D topological photonic states in all-dielectric photonics, and stimulate future synergy between subwavelength photonic topological materials and optoelectronics on PhC surfaces.

*Note added*: When this paper was under review for the final round, a proposal of type-II DPs in electronic materials with robust Fermi arcs, has appeared.^{48}

## Methods

### Symmetry transformation of photonic states

A photonic state \({\Psi _{n\vec k}}\left( {\vec r} \right)\) transforms under the \({\Theta _x} = {S_x} * {\cal T}\) operation as follows,

where \({\hat M_y}\) and \({\hat M_z}\) are the mirror transformation for the electric and magnetic fields:

and the operator \({\hat t_h}\) reverses the sign of the magnetic field. Acting Θ_{
x
} twice yields,

### Refraction

The photonic dispersion in the medium with refraction index *n*
_{
i
} is given by \(\omega = c\left| {\vec k} \right|{\rm{/}}{n_i}\). We consider a light beam injected from a medium with a refraction index *n*
_{
i
} > 1.65 into the PhC to enable frequency and wavevector matching with the Dirac cones. Around the DP at \({\vec k_0}\) = (*π*, *π*, *k*
_{0}), the dispersion in the medium can be expressed as \(\omega = c\left| {\vec k} \right|{\rm{/}}{n_i} = c\left| {{{\vec K}_0} + \vec q} \right|{\rm{/}}{n_i}\) where \(\vec q = \vec k - {\vec K_0}\). Since the perpendicular wavevector *k*
_{
z
} is not conserved during refraction, we can always set

for fixed *q*
_{||}, while adjusting *k*
_{
z
} to keep a constant frequency. The angle *ϕ*
_{
i
} is varied from 0 to 2*π*. The refraction in the *x*-*z* plane is determined by matching the frequency and the parallel wavevector, yielding

The perpendicular wavevector *q*
_{
z
} in the PhC is determined by the above equation, which has two solutions for *η* < −1

The refraction angle is determined through the group velocities in the PhC as, \({\theta _r} \equiv - {\rm{arctan}}\left( {\frac{{{v_x}}}{{{v_z}}}} \right)\). Using the dispersion in Eq. (5), we find that \({v_z} = v\left( {\eta + \frac{{\tau {q_z}}}{{\sqrt {{\gamma ^2}q_x^2 + q:z^2} }}} \right)\), \({v_x} = \frac{{\tau v\gamma {q_x}}}{{\sqrt {{\gamma ^2}q_x^2 + q:z^2} }}\). Inserting Eq. (12) into the definition of the refraction angle, we obtain

Refraction for generic \(\vec q\) (i.e., away from the *x*-*z* or *y*-*z* plane) is given in details in the Supplementary Materials.

### Calculation of surface states

The surface states are obtained by supercell calculations. The supercell is periodic in the *y*-*z* plane but finite in the *x* direction. There are seven layers of unit cell along this direction as sandwiched by air layers of length 3*a* on the left and right, separately. The simple cladding medium (air) used here is non-topological for all polarizations and useful to study topological surface states below the light-line. The supercell structure is set to preserve the *S*
_{
y
} symmetry. Since *S*
_{
y
} transforms (*k*
_{
y
}, *k*
_{
z
}) to (*k*
_{
y
}, −*k*
_{
z
}) in the surface BZ, the surface spectrum is symmetric with respect to *k*
_{
z
} = 0 and *k*
_{
z
} = *π*. In addition, the \({\cal T}\) symmetry guarantees that the surface spectrum is invariant under the transformation (*k*
_{
y
}, *k*
_{
z
}) to (−*k*
_{
y
}, −*k*
_{
z
}). Therefore the surface photonic dispersion is also symmetric with respect to *k*
_{
y
} = 0 and *k*
_{
y
} = *π*. As detailed in ref. 49, although there are other topological degeneracies in our PhC (such as nodal lines), they do not affect the surface states on the (100) and (010) surfaces.

In the calculation of the reference slab-defect states, we have set the permittivity of the slab-defect layer as *ε* = 8 (the same as that of the dielectric slab on top of the topological PhC). The logs of the woodpile PhCs above and below the slab-defect layer are of width 0.25*a*, height 0.3*a* and permittivity of 12 (silicon).

### Data availability

All relevant data is available from the corresponding author.

## Additional information

**Publisher’s note:** Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

## References

- 1.
Dirac, P. A. M. The quantum theory of the electron.

*Proc. Roy. Soc. A***117**, 610–624 (1928). - 2.
Hasan, M. Z. & Kane, C. L. Topological insulators.

*Rev. Mod. Phys.***82**, 3045–3067 (2010). - 3.
Qi, X.-L. & Zhang, S.-C. Topological insulators and superconductors.

*Rev. Mod. Phys.***83**, 1057–1110 (2011). - 4.
Vafek, O. & Vishwanath, A. Dirac fermions in solids: from high-

*T*_{ c }cuprates and graphene to topological insulators and Weyl semimetals.*Ann. Rev. Cond. Matt. Phys***5**, 83–112 (2014). - 5.
Haldane, F. D. M. & Raghu, S. Possible realization of directional optical waveguides in photonic crystals with broken time-reversal symmetry.

*Phys. Rev. Lett.***100**, 013904 (2008). - 6.
Lu, L., Joannopoulos, J. D. & Soljačić, M. Topological photonics.

*Nat. Photon***8**, 821–829 (2014). - 7.
Yang, Z. et al. Topological acoustics.

*Phys. Rev. Lett.***114**, 114301 (2015). - 8.
Xiao, M., Chen, W.-J., He, W.-Y. & Chan, C. T. Synthetic gauge flux and Weyl points in acoustic systems.

*Nat. Phys***11**, 920–924 (2015). - 9.
He, C. et al. Acoustic topological insulator and robust one-way sound transport.

*Nat. Phys***12**, 1124–1129 (2016). - 10.
Süsstrunk, R. & Huber, S. D. Observation of phononic helical edge states in a mechanical topological insulator.

*Science***349**, 47–50 (2015). - 11.
Rocklin, D. Z., Chen, B. G.-g, Falk, M., Vitelli, V. & Lubensky, T. C. Mechanical Weyl modes in topological Maxwell lattices.

*Phys. Rev. Lett.***116**, 135503 (2016). - 12.
Zhang, X. Observing Zitterbewegung for photons near the Dirac point of a two-dimensional photonic crystal.

*Phys. Rev. Lett.***100**, 113903 (2008). - 13.
Huang, X. Q., Lai, Y., Hang, Z. H., Zheng, H. H. & Chan, C. T. Dirac cones induced by accidental degeneracy in photonic crystals and zero-refractive-index materials.

*Nat. Mater.***10**, 582–586 (2011). - 14.
Rechtsman, M. C. et al. Strain-induced pseudomagnetic field and photonic Landau levels in dielectric structures.

*Nat. Photon***7**, 153–158 (2013). - 15.
Khanikaev, A. B. et al. Photonic topological insulators.

*Nat. Mater.***12**, 233–239 (2013). - 16.
Chen, W.-J., Jiang, S.-J., Chen, X.-D., Dong, J.-W. & Chan, C. T. Experimental realization of photonic topological insulator in a uniaxial metacrystal waveguide.

*Nat. Commun.***5**, 5782 (2014). - 17.
Ma, T., Khanikaev, A. B., Mousavi, S. H. & Shvets, G. Guiding electromagnetic waves around sharp corners: topologically protected photonic transport in metawaveguides.

*Phys. Rev. Lett.***114**, 127401 (2015). - 18.
Wu, L.-H. & Hu, X. Scheme for achieving a topological photonic crystal by using dielectric material.

*Phys. Rev. Lett.***114**, 223901 (2015). - 19.
Xu, L., Wang, H.-X., Xu, Y. D., Chen, H. Y. & Jiang, J.-H. Accidental degeneracy in photonic bands and topological phase transitions in two-dimensional core-shell dielectric photonic crystals.

*Opt. Express.***24**, 18059–18071 (2016). - 20.
Wang, Z., Chong, Y., Joannopoulos, J. D. & Soljačić, M. Observation of unidirectional backscattering-immune topological electromagnetic states.

*Nature***461**, 772–775 (2009). - 21.
Poo, Y., Wu, R.-X., Lin, Z., Yang, Y. & Chan, C. T. Experimental realization of self-guiding unidirectional electromagnetic edge states.

*Phys. Rev. Lett.***106**, 093903 (2011). - 22.
Hafezi, M., Mittal, S., Fan, J., Migdall, A. & Taylor, J. Imaging topological edge states in silicon photonics.

*Nat. Photon***7**, 1001–1005 (2013). - 23.
Rechtsman, M. C. et al. Photonic Floquet topological insulators.

*Nature***496**, 196–200 (2013). - 24.
Mittal, S., Ganeshan, S., Fan, J., Vaezi, A. & Hafezi, M. Measurement of topological invariants in a 2D photonic system.

*Nat. Photon***10**, 180–183 (2016). - 25.
Lu, L., Fu, L., Joannopoulos, J. D. & Soljačić, M. Weyl points and line nodes in gyroid photonic crystals.

*Nat. Photon***7**, 294–299 (2013). - 26.
Lu, L. et al. Experimental observation of Weyl points.

*Science***349**, 622–624 (2015). - 27.
Gao, W. et al. Plasmon Weyl degeneracies in magnetized plasma.

*Nat. Comm***7**, 12435 (2016). - 28.
Chen, W.-J., Xiao, M. & Chan, C. T. Experimental observation of robust surface states on photonic crystals possessing single and double Weyl points.

*Nat. Commun.***7**, 13038 (2016). - 29.
Wang, H.-X., Xu, L., Chen, H. Y. & Jiang, J.-H. Three-dimensional photonic Dirac points stabilized by point group symmetry.

*Phys. Rev. B***93**, 235155 (2016). - 30.
Xiao, M., Lin, Q. & Fan, S. Hyperbolic Weyl point in reciprocal chiral metamaterials.

*Phys. Rev. Lett.***117**, 057401 (2016). - 31.
Lu, L. et al. Symmetry-protected topological photonic crystal in three dimensions.

*Nat. Phys***12**, 337–340 (2016). - 32.
Slobozhanyuk, A. et al. Three-dimensional all-dielectric photonic topological insulator.

*Nat. Photon***11**, 130–136 (2017). - 33.
Fu, L. & Kane, C. L. Topological insulators with inversion symmetry.

*Phys. Rev. B***76**, 045302 (2007). - 34.
Soluyanov, A. A. et al. Type-II Weyl semimetals.

*Nature***527**, 495–498 (2015). - 35.
Xu, Y., Zhang, F. & Zhang, C. Structured Weyl points in spin-orbit coupled fermionic superfluids.

*Phys. Rev. Lett.***115**, 265304 (2015). - 36.
König, A. & Mermin, N. D. Electronic level degeneracy in nonsymmorphic periodic or aperiodic crystals.

*Phys. Rev. B***56**, 13607–13610 (1997). - 37.
Parameswaran, S. A., Turner, A. M., Arovas, D. P. & Vishwanath, A. Topological order and absence of band insulators at integer filling in non-symmorphic crystals.

*Nat. Phys.***9**, 299–303 (2013). - 38.
Lee, J.-H. et al. Layer-by-layer photonic crystal fabricated by low-temperature atomic layer deposition.

*Appl. Phys. Lett.***90**, 151101 (2007). - 39.
Deubel, M. et al. Direct laser writing of three-dimensional photonic-crystal templates for telecommunications.

*Nat. Mater.***3**, 444–447 (2004). - 40.
Yang, B.-J., Morimoto, T. & Furusaki, A. Topological charges of three-dimensional Dirac semimetals with rotation symmetry.

*Phys. Rev. B***92**, 165120 (2015). - 41.
Morimoto, T. & Furusaki, A. Weyl and Dirac semimetals with

*Z*_{2}topological charge.*Phys. Rev. B***89**, 235127 (2014). - 42.
John, S. & Yang, S. Electromagnetically Induced Exciton Mobility in a Photonic Band Gap.

*Phys. Rev. Lett.***99**, 046801 (2007). - 43.
Ishizaki, K. & Noda, S. Manipulation of photons at the surface of three-dimensional photonic crystals.

*Nature***460**, 367–370 (2009). - 44.
Joannopoulos, J. D., Johnson, S. G., Winn, J. N. & Meade, R. D.

*Photonic Crystals: Molding the Flow of Light*(Princeton University Press, 2008). - 45.
Luo, J., Xu, P., Sun, T. & Gao, L. Tunable beam splitting and negative refraction in heterostructure with metamaterial.

*Appl. Phys. A***104**, 1137–1142 (2011). - 46.
Fu, L. Topological crystalline insulators.

*Phys. Rev. Lett.***106**, 106802 (2011). - 47.
Fu, L. & Kane, C. L. Topology, delocalization via average symmetry and the symplectic Anderson transition.

*Phys. Rev. Lett.***109**, 246605 (2012). - 48.
Chang, T.-R. et al. Type-II symmetry-protected topological Dirac semimetals.

*Phys. Rev. Lett.***119**, 026404 (2017). - 49.
Wang, H.-X., Chen, Y., Hang, Z. H., Kee, H.-Y. & Jiang, J.-H. 3D

*Z*_{2}topological nodes in nonsymmorphic photonic crystals: ultrastrong coupling and anomalous refraction. preprint at https://arxiv.org/abs/1608.02437.

## Acknowledgements

We thank Sajeev John, Zhengyou Liu, Ling Lu, Chen Fang, Huanyang Chen, Yun Lai, Chunying Qiu, and Jie Luo for many inspiring discussions. H.X.W and J.H.J acknowledge supports from the National Science Foundation of China (Grant no. 11675116) and the Soochow university. Z.H.H is supported by National Science Foundation of China (Grant no. 11574226). Y.C and H.Y.K are supported by NSERC of Canada and Center for Quantum Materials at the University of Toronto.

## Author information

### Author notes

Hai-Xiao Wang and Yige Chen contributed equally to this work

### Affiliations

#### College of Physics, Optoelectronics and Energy, & Collaborative Innovation Center of Suzhou Nano Science and Technology, Soochow University, 1 Shizi Street, Suzhou, 215006, China

- Hai-Xiao Wang
- , Zhi Hong Hang
- & Jian-Hua Jiang

#### Department of Physics, University of Toronto, Toronto, M5S 1A7, Canada

- Yige Chen
- & Hae-Young Kee

#### Canadian Institute for Advanced Research, Toronto, ON, M5G 1Z8, Canada

- Hae-Young Kee

### Authors

### Search for Hai-Xiao Wang in:

### Search for Yige Chen in:

### Search for Zhi Hong Hang in:

### Search for Hae-Young Kee in:

### Search for Jian-Hua Jiang in:

### Contributions

J.H.J conceived the idea and wrote the manuscript. J.H.J and Z.H.H designed the photonic architecture. H.X.W, Y.C, H.Y.K and J.H.J did the theoretical analysis and calculations. J.H.J guided the research.

### Competing interests

The authors declare no competing financial interests.

### Corresponding authors

Correspondence to Hae-Young Kee or Jian-Hua Jiang.

## Electronic supplementary material

## Rights and permissions

**Open Access** This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.